New Quaternary Rare-Earth Chalcogenides BaLnSn2Q6 (Ln = Ce, Pr, Nd, Q = S; Ln = Ce, Q = Se): Synthesis, Structure, and Magnetic Properties.
Feng, Kai; Zhang, Xu; Yin, Wenlong; Shi, Youguo; Yao, Jiyong; Wu, Yicheng; Inorganic chemistry 53 (2014) 2248–2253; doi:10.1021/ic402934m

data_4337239
_publ_section_title
;
 New Quaternary Rare-Earth Chalcogenides BaLnSn2Q6 (Ln = Ce, Pr, Nd, Q =
 S; Ln = Ce, Q = Se): Synthesis, Structure, and Magnetic Properties.
;
_journal_issue                   4
_journal_name_full               'Inorganic chemistry'
_journal_page_first              2248
_journal_page_last               2253
_journal_paper_doi               10.1021/ic402934m
_journal_volume                  53
_journal_year                    2014
_chemical_formula_sum            'Ba Nd S6 Sn2'
_chemical_formula_weight         711.32
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           26
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2c -2'
_symmetry_space_group_name_H-M   'P m c 21'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   4.0098(8)
_cell_length_b                   19.761(4)
_cell_length_c                   11.841(2)
_cell_measurement_reflns_used    4221
_cell_measurement_temperature    153(2)
_cell_measurement_theta_max      31.4919
_cell_measurement_theta_min      2.6850
_cell_volume                     938.3(3)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 2008)'
_computing_publication_material  Diamond
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      153(2)
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Rigaku AFC10 diffractometer'
_diffrn_measurement_method       dtprofit.ref
_diffrn_radiation_monochromator  'Graphite Monochromator'
_diffrn_radiation_source         'Rotating Anode'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0325
_diffrn_reflns_av_sigmaI/netI    0.0338
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            6419
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         2.06
_exptl_absorpt_coefficient_mu    16.100
_exptl_absorpt_correction_T_max  0.120
_exptl_absorpt_correction_T_min  0.071
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed'
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    5.036
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Chip
_exptl_crystal_F_000             1248
_exptl_crystal_size_max          0.1750
_exptl_crystal_size_mid          0.1450
_exptl_crystal_size_min          0.1350
_refine_diff_density_max         3.700
_refine_diff_density_min         -1.721
_refine_diff_density_rms         0.291
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.24(3)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.057
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     122
_refine_ls_number_reflns         1991
_refine_ls_number_restraints     13
_refine_ls_restrained_S_all      1.090
_refine_ls_R_factor_all          0.0284
_refine_ls_R_factor_gt           0.0280
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0300P)^2^+13.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0656
_refine_ls_wR_factor_ref         0.0659
_reflns_number_gt                1973
_reflns_number_total             1991
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic402934m_si_001.cif
_cod_data_source_block           BaNdSn2S6
_cod_original_cell_volume        938.2(3)
_cod_original_sg_symbol_H-M      Pmc21
_cod_database_code               4337239